Volvo accelerated corrosion test
Volvo also Refer to this test as ACT -1.
This standard defines an accelerated corrosion test method to be used in assessing the corrosion resistance of metals in environments where there is a significant influence of chloride ions, mainly as sodium chloride from a marine source or by winter road de-icing salt. It specifies a test procedure to be used in conducting the accelerated corrosion test to simulate atmospheric corrosion conditions in a controlled way.
The one-week main test cycle is composed of two twelve-hour sub-cycles, one with controlled humidity cycling; sub-cycle 1, the other including salt solution application, sub-cycle 2.
Sub cycle 1 requires constant conditions at 35°C & 95% RH for 4 h, followed by an increase of temperature to 45°C whilst reducing the humidity to 50% over a 2 hour period. This is followed by constant conditions of 45°C & 50% RH for 4 h, together with a 2 hour period of 35°C & 95%RH. Step 1:4) Temperature decrease from 45°C to 35°C.
Sub cycle 2 requires spraying with salt solution for 15 mins then keeping the samples at 35°C for 1 h 45 min whilst maintaining a set point of 95% – 99% RH in such a way that the test objects remain wet. These steps are repeated in sequence to give a total period of 6 hours. Drying at 45°C & 50% RH for a 2 hour period followed by a further 2 hour period of 35°C whilst maintaining 95% RH.
Necessary cookies are absolutely essential for the website to function properly. This category only includes cookies that ensures basic functionalities and security features of the website. These cookies do not store any personal information.
Any cookies that may not be particularly necessary for the website to function and is used specifically to collect user personal data via analytics, ads, other embedded contents are termed as non-necessary cookies. It is mandatory to procure user consent prior to running these cookies on your website.